# DESIGN OF LAMINATES FOR IN-PLANE LOADING

Save this PDF as:

Size: px
Start display at page:

Download "DESIGN OF LAMINATES FOR IN-PLANE LOADING"

## Transcription

1 DESIGN OF LAMINATES FOR IN-PLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, Le Mans, France SUMMARY This work relates to the design of laminated structures primarily loaded in membrane, such as pressure vessels. It derives complete formulas, i.e. valid for any loading and any laminate, and without any approximation. Using the so called material ratio and the loading ratio, the design criterion takes a very simple form, equating the two ratios. Keywords: design, laminate, netting theory, polar description of anisotropy, anisotropy. INTRODUCTION Structures primarily loaded in membrane, such as cylindrical pressure vessels, must certainly been considered as the simplest case for design. However even for such cases, the tools available to the designer are on one side the netting theory (NT), which provides explicit design factors but is known to be approximate, and on the other side the classical laminated plate theory (CLPT), which is a precise analysis method, but so requires an iterative process to contribute to a design. As the CLPT in its usual form involves huge algebraic manipulations, it is not possible to derive explicit formulas even for simple cases such as pressurized tubes and only numerical computations can be done. These numerical applications of the CLPT are of course very easy to do and show discrepancy between this CLPT and the netting theory but might not reveal the significant factors for the design. Surprisingly, no work seems to have faced this question of significant parameters until 2002 when Evans and Gibson [1] gave a clear insight into the problem. In order to reveal the factors involved, they succeeded in developing explicit formulas based on the CLPT and compared them to the netting analysis for balanced angle-ply laminated tubes with hoop-to-axial-stress ratio of 2:1. They have shown that part of the netting theory can be retained (the principal strains of the plies should be equal), while other parts need to be corrected and they gave a correction formula for the optimal ply angle. Although they had to do lots of tedious algebraic manipulations (Evans [2]), their formulas do not solve exactly the CLPT equations, due to the cumbersome algebra involved in the theory, so their results for the correction in the angle still retain a difference with full calculation. In the numerical examples they published, this correction is shown to be small, however its small value is not guaranteed for other cases and the challenge for an exact CLPT solution remains. To summarize, the limitations of the paper of Evans and Gibson are the following: i) they limited to angleply laminates, ii) they limited to a 2:1 ratio for the principal stresses, iii) their formulas are approximate.

2 METHODOLOGY AND HYPOTHESES For many years, the author has developed the so-called polar method for twodimensional continuum mechanics, using as variables the polar parameters, which are complex linear combinations of the Cartesian components of the stress, strain, stiffness, compliance or other tensors. Among other features, it provides an efficient description of plane anisotropy. So it is useful for two-dimensional anisotropic systems such as composite materials. Specially, using these parameters, the CLPT receives an equivalent but simpler form, which makes possible many explicit algebraic developments otherwise intractable. From this, many applications can be derived for analysis and also for design of composites (see for instance [3]). This method was used in the present research, with the aim to improve the results of Evans and Gibson, and suppress their drawbacks. In this part of the paper, we will first describe the loading, geometric and material hypotheses of the study, present some important points of the polar method, then introduce two ratios which are relevant for the present research. In the next part, rules of design will be given, and the design criterion will be derived from them. Structural hypotheses We limit to the simplest conditions for the structure to be designed. Material and geometric hypotheses: the structure is -or behaves like- a laminated plate. with zero coupling stiffnesses and orthotropic membrane stiffnesses. We will specially consider laminates made of identical plies. Loading hypotheses: the structure is loaded in membrane, with uniform membrane forces N ij. The principal loads are N 1 and N 2, and we limit to the cases with N 1 > N 2 > 0. These hypotheses are those of the netting theory, and notably apply to pressure vessels. Extensions can be made but are not presented here as they make more intricate the discussion, which might conceal the principles of the method, that we want to emphasize. Basics of the polar method Complete equations can be found in [3]. A simpler form is sufficient in the present study. They are presented here in the case of orthotropy and in the principal axes of stress, strain or stiffness: for the stresses or membrane forces, they are obtained from the principal values with major principal axis along direction 1 as: 2 T N 1 N 2 2 R N 1 N 2 and similarly for the strains: 2 t r 1 2

3 for membrane stiffnesses with major principal axis in direction 1, they are: 8 T 0 A A A 1212 A A A 1122 A R 0 A A A 1212 A A 1111 A 2222 Similar formulas hold for ply stiffnesses and for compliances. Loading ratio A loading ratio is defined from the principal membrane forces N 1 > N 2 > 0 as: R T N 1 N 2. N 1 N 2 This quantity will prove to be more relevant to structural design than the more usual ratio N 1/ N 2 (which is the hoop-to-axial-stress ratio for tubes studied by Evans and Gibson). With the assumed values for the principal loads N k, this material ratio is positive and less than 1. It equals 1/3 in the classical case of cylindrical pressure vessel with hoop-to-axial-stress ratio equal to 2. Material ratio for the laminate With A ijkl being the in-plane stiffnesses, the (in-plane) orthotropy axes of the laminate are (1, 2) with the first axis along the direction of the major stiffness: A 1111 > A A material ratio is then defined from two of the polar parameters, as: A 1111 A 2222 A A 1122 A It should be noted that this material ratio does not involve the shear stiffness A Material ratio for a ply A material ratio for any ply is defined similarly from the stiffnesses Q ijkl in the material orthotropy axes (L, T) of the ply : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT This ratio can also be expressed with the compliances S ijkl in the same material orthotropy axes (L, T) or the engineering constants, longitudinal and transverse Young's moduli and, and principal (major) Poisson's ratio ν LT : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT S TTTT S LLLL S LLLL 2 S LLTT S TTTT E 2 LT Notice that this material ratio does not involve the shear property in the orthotropy axes.

4 OVERALL DESIGN PROCESS Design process is split in two steps: first at the laminate level, an overall material satisfying the loading conditions is built, and second, a convenient stacking giving the required overall properties is searched for. Both steps involve the ratios introduced above. Overall design rules We use as overall design criterion the following empirical rules, closely related to the guidelines of the netting analysis: i) select an orthotropic laminate with the major principal axis of stiffness aligned with the major principal axis of the loads, ii) select the material so that the strain is isotropic. Design based on these rules will be consequently called orthotropic isostrain design. Comments of the overall design rules These two rules are neither arbitrary nor obvious. Notice that they do not refer to a definite objective, and are not derived theoretically but are empirical, and so have to be assessed from their consequences. However some rationale is of course behind them. Starting with the meaning of the first rule, it is certainly common sense to retain orthotropic materials with axes aligned with the directions of principal stresses: as the stresses (being a second order tensor) have two orthogonal directions of symmetry, so should have the overall stiffnesses, i.e. the material should be orthotropic (for in-plane stiffness properties). Further, the first rule requires that the major orthotropy axis should be along the highest stress and the minor along the lowest stress (remember that the major stiffness is not always along the major stiffness axis, as it may be off-axis, however the stiffness along the major orthotropy axis is always highest than that along the minor orthotropy axis). This point may appear questionable when comparing to the principles of the netting theory, which aims to optimize the structural strength (and in fact cannot meet exactly its assumptions and its aim), while the present formulation appears to rest on elastic behaviour rather to strength behaviour: it is a fact that for an arbitrary orthotropic material, strength and stiffness may differ in orientation and variation. Results for laminates will justify afterwards this rule together with the second rule. As a consequence of the first rule, the strains have the same principal axes than the stresses and stiffnesses, but the major strain may be along any of the principal axes. The second rule settles this point as its meaning is the following: the material should be strained at the same level in any of the principal axes, and consequently in any direction. This second rule is specially relevant for laminates made of identical plies. According to the CLPT, while the state of strain (for membrane loading) is the same through the thickness in the structure axes, it generally varies from ply to ply in the local axes (principal axes of the plies), and so the state of stress in each ply depends on the ply

5 orientation (whatever the axes considered). Only in the case of an isotropic state of strain, the strains are the same in every ply whatever the axes, and consequently the states of stress are the same in the local axes of all the plies: then, every ply is in the same state of strain and stress and so contributes equally to the structural behaviour, which is certainly a good design (and probably an optimal design). Formula of the overall design criterion Translating the design rules in equations is quite simple using the polar parameters. For an orthotropic material loaded in its symmetry axes, the stress-strain relationship, expressed in these symmetry axes with polar parameters, writes: T 4 t 4 r R 4 t 2 T 0 R 0 r Then we have to state that the overall strain is isotropic, that is: r 0 Eliminating t, this gives the design criterion, which expresses simply as the equality of the load and material ratios defined above: R T. The reader can check that this can be derived using the Cartesian components in the orthotropy axes, at the cost of more algebra. STACKING DESIGN PROCESS The previous step of design has defined an overall condition for the material: it must be orthotropic for in-plane stiffness, with a fixed value of its material ratio. The next step will be to find stacking sequences meeting these requirements. As an orthotropic laminate possesses 4 independent in-plane stiffness parameters, while the material ratio involves only 2 of these parameters, it can be guessed that there might be several solutions. In the following, we examine the common (and simplest) case when the laminate is made of identical plies. Polar method applied to CLPT For laminates made of identical plies, the CLPT equations receive a very simple form with the polar parameters (see [3]). We limit here to the orthotropic case useful for the present research. In this case the 4 polar in-plane stiffness parameters have very simple expressions as functions of the polar parameters of the ply. Specially: T t 1 t R 1 cos 2 N k k 1 N

6 where t is the laminate thickness, N is the number of layers and θ k the orientation of the k layer. Consequently, the material ratio of the laminate is equal to the material ratio for the plies /, multiplied by a weighting factor: 1 N N cos2 k k1 It should be noticed that the weighting factor is always less than one. Stacking design equation Substituting in the last equation the value of the loading ratio gives the design equation: R T 1 T N cos 2 1 N k k 1 This equation involves three quantities, the loading ratio of the structure, the material ratio of the ply, and the weighting factor of the stacking sequence. Comments of the stacking design equation The conditions of applicability of our design process appear from this stacking design equation. As the weighting factor is less than 1, solutions can be expected only when: the loading factor should be less than the ply material factor and be at most equal, in which case the only possible solution is a unidirectional material. It can be shown from stability consideration that the material ratio of any material is also less than 1. Table 1 shows typical values for usual unidirectional composites. Table1 : Typical values of the ply material ratio / and polar stiffness parameters for unidirectional reinforcement (T 0,, R 0, in GPa). Material (V f 60%) / T 0 R 0 E-glass /epoxyde HT-carbon /epoxyde HM-carbon /epoxyde The material ratio has two effects. First, when it increases, the range of possible loading is increased too. As said above, the loading ratio range extends to the value of the material ratio, but the effect appears even larger when considering the ratio of the

7 principal stresses instead of the loading ratio. For instance, changing from glass/epoxy plies to HM carbon/epoxy plies increases the material ratio by 40%, and so is the loading ratio range, while the range for the principal stresses ratio is increased by 140%, from 3.8 up to 9. It also can be shown that when the material ratio increases, the formulas get closer to the netting analysis results, and when it goes up to 1, all the formulas reduce to the netting analysis. Using micromechanics formulas of prediction of elastic properties of UD shows that the material ratio is closely dependent on the reinforcement-to-matrix-stiffness ratio (such as E f /E m ): when this ratio increases, so does the material ratio / of a unidirectionally reinforced ply, up to the limiting case of a very soft matrix (for instance, rubber reinforced with steel fibres), with the ratio going up to 1. Plies reinforced with balanced fabrics have a zero material ratio and cannot be used in our design method. Plies reinforced with unbalanced fabrics have generally a low material ratio, limiting the range of loading they can efficiently carry. When the conditions of applicability are met, several solutions generally exist. The weighting factor should receive a fixed value equal to the loading ratio divided by the ply material ratio, and as it includes an unspecified number N of parameters θ k, an infinite number of solutions exist theoretically. Practical conditions on the number N and the angles values reduce the effective solutions. APPLICATION EXAMPLES To go further, the practical field of design parameters must be specified. Angle-ply and cross-ply laminates are of interest. Design of cylindrical pressure vessel is also of major importance for its practical applications as well as for comparison purpose with the netting theory and the Evans and Gibson results. Design with angle-ply laminates Angle-ply laminates with layers at ±β (or filament winding in these same directions) are defined by a unique parameter and the design equation writes: cos 2 R T This equation can be solved in seconds with a pocket calculator, to give the optimal angle in agreement with the CLPT. The influence of the significant factors can be check easily. The design angle ±β 0 of the netting theory is given by the limit case when the material ratio equals 1: cos 2 0 R T

8 It appears that cos 2 cos 2 0 so the exact angle is closer to the major stress direction than predicted by the netting theory. A quantitative comparison between these angle values can be obtained by Taylor expansion up to the second order in the quantity ( - )/. It gives: 1 1 T /R T 0 1 T /R or using the principal Young's moduli and Poisson's ratio: 1 0 T /R LT 1 1 T / R third order 1 LT third order Design with cross-ply laminates Cross-ply laminates are also defined by only one parameter 0 < q < 1, the percentage q of layers at 0, with 1-q layers at 90. The design equation writes: 2 q 1 R T So the percentage of plies at 0 should be higher than that indicated by the netting theory, which is such as 2 q 0 1 R /T. Design of cylindrical pressure vessel For cylindrical pressure vessels, N 1 2 N 2, so T 3R. These values in the formulas derived above for angle-ply laminates define the exact value of the helical angles at which such cylindrical pressure vessels must be wound, angles which are closer to the hoop direction than predicted by the netting theory. The approximate formula derived by Evans and Gibson writes: LT while the present analysis gives: LT LT third order The main difference comes from the term instead of -, which appears in the denominator of the Evans and Gibson formula. It explain about 90% of the difference they observed with the numerical results they computed from the CLPT. With the second order terms (in the parentheses) of the present analysis, the CLPT values are recovered exactly.

9 CONCLUSION Within the conditions of applicability of the present approach, all the limitations of the analysis of Evans and Gibson are relieved and explicit design formulas for any state of stress and stacking sequence can be derived. A further step in this research will be to study the stability of solutions obtained. References 1. J T Evans and A G Gibson, 2002, Composite angle ply laminates and netting analysis, Proc. R. Soc. Lond., Vol A 458, pp J T Evans, 2007, private communication ( dated July 6 th, 2007). 3. G Verchery, 1999, Designing with anisotropy, keynote lecture, Twelfth International Conference on Composite Materials (ICCM-12), 5-9 July, Paris.

### LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS

XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds

More information

### DESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION

DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place

More information

### QUESTION BANK Composite Materials

QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.

More information

### 3D and Planar Constitutive Relations

3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace

More information

### Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA

Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from

More information

### Bending of Simply Supported Isotropic and Composite Laminate Plates

Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto Gutierrez-Miravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,

More information

### Chapter 2 - Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.

Chapter - Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.

More information

### Understand basic stress-strain response of engineering materials.

Module 3 Constitutive quations Learning Objectives Understand basic stress-strain response of engineering materials. Quantify the linear elastic stress-strain response in terms of tensorial quantities

More information

### Lectures on. Constitutive Modelling of Arteries. Ray Ogden

Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics

More information

### LAMINATED COMPOSITE PLATES

LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended

More information

### Stacking sequences for Extensionally Isotropic, Fully Isotropic and Quasi-Homogeneous Orthotropic Laminates.

49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 7-10 April 2008, Schaumburg, IL AIAA 2008-1940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and Quasi-Homogeneous

More information

### A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks

Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints

More information

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional

More information

### EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING

Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 5-22 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,

More information

### Passive Damping Characteristics of Carbon Epoxy Composite Plates

Journal of aterials Science and Engineering A 6 (1-2) (2016) 35-42 doi: 10.17265/2161-6213/2016.1-2.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K

More information

### 2.1 Strain energy functions for incompressible materials

Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to

More information

### USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE

Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and

More information

### MATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f

MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown

More information

### FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.

FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT - Institut Supérieur de l Automobile et des Transports, LRMA - Laboratoire de

More information

### Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains

Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model

More information

### ME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)

ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,

More information

### Finite element modelling of infinitely wide Angle-ply FRP. laminates

www.ijaser.com 2012 by the authors Licensee IJASER- Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angle-ply FRP laminates

More information

### Non-conventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France

20 th International Conference on Composite Materials Copenhagen, 19-24th July 2015 Non-conventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi

More information

### ISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013

Delamination Studies in Fibre-Reinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering

More information

### MATERIAL ELASTIC ANISOTROPIC command

MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The

More information

### Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37

Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREE-DIMENSIONAL, TIME- DEPENDENT, NON-LINEAR, UNI-DIRECTIONAL

More information

### S. Srinivasan, Technip Offshore, Inc., Houston, TX

9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENT-WOUND GLASS-FIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING

More information

### APPLICATION OF ISOTENSOID-BASED CROSS SECTIONS TO FILAMENT-WOUND TOROIDAL PRESSURE VESSELS

APPLICATION OF ISOTENSOID-BASED CROSS SECTIONS TO FILAMENT-WOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering

More information

### DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS

DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the

More information

### Tensile behaviour of anti-symmetric CFRP composite

Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of anti-symmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b

More information

### 2. Mechanics of Materials: Strain. 3. Hookes's Law

Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate

More information

### Enhancing Prediction Accuracy In Sift Theory

18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department

More information

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional

More information

### MODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations

MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic

More information

### MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP

16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic

More information

### Continuum Mechanics. Continuum Mechanics and Constitutive Equations

Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform

More information

### EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES

EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC

More information

### BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS

BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6-13-1, Ohsawa, Mitaka,

More information

### CORRELATING OFF-AXIS TENSION TESTS TO SHEAR MODULUS OF WOOD-BASED PANELS

CORRELATING OFF-AXIS TENSION TESTS TO SHEAR MODULUS OF WOOD-BASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating off-axis modulus of elasticity

More information

### THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH

THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk

More information

### STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK

THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information

More information

### A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms

A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms

More information

### PEAT SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity

PEAT8002 - SEISMOLOGY Lecture 9: Anisotropy, attenuation and anelasticity Nick Rawlinson Research School of Earth Sciences Australian National University Anisotropy Introduction Most of the theoretical

More information

### Composite Laminate Modeling

omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER

More information

### Fracture Mechanics of Composites with Residual Thermal Stresses

J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate

More information

### ANALYSES OF COMPOSITE STRUCTURES. by Stephen W. Tsai, Donald F, Adams, and Douglas R. Doner NASA CR-620 REPORT

NASA CONTRACTOR REPORT NASA CR-620 -sa: 19960410 079 ANALYSES OF COMPOSITE STRUCTURES by Stephen W. Tsai, Donald F, Adams, and Douglas R. Doner & Prepared by PHILCO CORPORATION Newport Beach, Calif. for

More information

### University of Bristol - Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified

Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.

More information

### VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 )

VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials

More information

### SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS

Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 79-85 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University

More information

### PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses

OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 24-10-02

More information

### 2D damping predictions of fiber composite plates: Layup effects

Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite

More information

### Poisson s ratio as a sensitive indicator of (fatigue) damage in fibre-reinforced plastics

10.1111/j.1460-2695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibre-reinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department

More information

### COMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS

6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 15-16 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania

More information

### Analysis of high loss viscoelastic composites

Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science

More information

### Continuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms

Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive

More information

### Mechanics of Irregular Honeycomb Structures

Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International

More information

### ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES

NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,

More information

### EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTI-SCALE ANALYSIS

THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTI-SCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu

More information

### Aspect Ratio Requirements for Nanotube-Reinforced, Polymer-Matrix Composites

Aspect Ratio Requirements for Nanotube-Reinforced, Polymer-Matrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a

More information

### Stress-Strain Behavior

Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

More information

### Modeling of Fiber-Reinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014

Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of Fiber-Reinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter

More information

### Micro-meso draping modelling of non-crimp fabrics

Micro-meso draping modelling of non-crimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Non-crimp fabrics (NCFs) are

More information

### COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)

Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design

More information

### PLAT DAN CANGKANG (TKS 4219)

PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, two-dimensional structural components of which

More information

### A simple plane-strain solution for functionally graded multilayered isotropic cylinders

Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000-000 1 A simple plane-strain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The

More information

### Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling

Mathematical Modeling of Displacements and Thermal Stresses in Anisotropic Materials (Sapphire) in Cooling Timo Tiihonen & Tero Tuovinen September 11, 2015 European Study Group with Industry, ESGI 112,

More information

### Semi-Membrane and Effective Length Theory of Hybrid Anisotropic Materials

International Journal of Composite Materials 2017, 7(3): 103-114 DOI: 10.5923/j.cmaterials.20170703.03 Semi-Membrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju

More information

### IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF

V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS

More information

### PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES

THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile

More information

### SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS

SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATEC-SP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS

More information

### CHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS

CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress

More information

### Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE

1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for

More information

### Stresses and Strains in flexible Pavements

Stresses and Strains in flexible Pavements Multi Layered Elastic System Assumptions in Multi Layered Elastic Systems The material properties of each layer are homogeneous property at point A i is the same

More information

### Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites

Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.61-67, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.

More information

### Presented By: EAS 6939 Aerospace Structural Composites

A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have

More information

### Anisotropic modeling of short fibers reinforced thermoplastics materials with LS-DYNA

Anisotropic modeling of short fibers reinforced thermoplastics materials with LS-DYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics

More information

### BUCKLING AND POST-BUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION

2 th International Conference on Composite Materials Copenhagen, 19-24 th July 215 BUCKLING AND POST-BUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.

More information

### A copy can be downloaded for personal non-commercial research or study, without prior permission or charge

York, C. (2015) On tapered warp-free laminates with single-ply terminations. Composites Part A: Applied Science and Manufacturing, 72, pp. 127-138. Copyright 2015 Elsevier Ltd. A copy can be downloaded

More information

### CONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS

Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical

More information

### Mechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total

Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the

More information

### CSMA Introduction. M. Brunetti 1, A. Vincenti 2, S. Vidoli 3

CS017 13ème Colloque National en Calcul des Structures 15-19 Mai 017, Presqu île de Giens (Var) 13ème Colloque National en Calcul des Structures Multistable shell structures satisfying clamped boundary

More information

### Chapter 1 -- Introduction

Chapter 1 -- Introduction 1.1 Aft pressure bulkhead On a large transport aircraft, the pressurized cabin is closed at the aft end by a domeshaped pressure bulkhead as is shown in Fig. 1.1. In general,

More information

### Machine Direction Strength Theory of Corrugated Fiberboard

Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,

More information

### Frequency Response of Composite Laminates at Various Boundary Conditions

International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.11-15 Frequency Response of Composite Laminates at Various Boundary Conditions

More information

### Basic Energy Principles in Stiffness Analysis

Basic Energy Principles in Stiffness Analysis Stress-Strain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting

More information

### Gerald Allen Cohen, 83, passed away Oct. 1, 2014, at his home in Laguna Beach.

Dr Gerald Allen Cohen (1931-2014) Ring-stiffened shallow conical shell designed with the use of FASOR for NASA s Viking project in the 1970s. (from NASA TN D-7853, 1975, by Walter L. Heard, Jr., Melvin

More information

### USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR

USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree

More information

### A Finite Element Model for Numerical Analysis of Sintering

A Finite Element Model for Numerical Analysis of Sintering DANIELA CÂRSTEA High-School Group of Railways, Craiova ION CÂRSTEA Department of Computer Engineering and Communication University of Craiova

More information

### Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials

Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected

More information

### Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading

Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering

More information

### UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.

UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude

More information

### MECHANICS OF MATERIALS

Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:

More information

### Malaysia Phone: ; Fax:

International Conference on Mechanical Engineering Research (ICMER013), 1-3 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia

More information

### Generic Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials

University of Nebraska - Lincoln DigitalCommons@University of Nebraska - Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 12-9-2011 Generic

More information

### International Journal of Advanced Engineering Technology E-ISSN

Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,

More information

### Plane Strain Test for Metal Sheet Characterization

Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and Anne-Marie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS - Cachan, Avenue

More information

### Bilinear Modelling of Cellulosic Orthotropic Nonlinear Materials

Bilinear Modelling of Cellulosic Orthotropic Nonlinear Materials E.P. SALIKLIS, T.J. URBANIK and B. TOKYAY The proposed method of modelling orthotropic solids that have a nonlinear constitutive material

More information

### MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS

MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.-X. Irisarri, J.-F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francois-xavier.irisarri@onera.fr,

More information

### 2 To whom all correspondences should be addressed:

Composite Modeling and Analysis of FDM Prototypes for Design and Fabrication of Functionally Graded Parts Longmei Li, Q. Sun, C. Bellehumeur 1,andP.Gu 2 Department of Mechanical and Manufacturing Engineering

More information

### Game Physics. Game and Media Technology Master Program - Utrecht University. Dr. Nicolas Pronost

Game and Media Technology Master Program - Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit

More information